AISI 1020 Low Carbon.docx
AISI 102 Low Carbon Steel...
AISI 1020 Low Carbon/Low Tensile Steel Introduction AISI 1020 is a low hardenability and low tensile carbon steel with Brinell hardness of 119 – 235 and tensile strength of 410-790 MPa. It has high machinability, high strength, high ductility and good weldability. It is normally used in turned and polished or cold drawn condition. Due to its low carbon content, it is resistant to induction hardening or flame hardening. Due to lack of alloying elements, it will not respond to nitriding. However, carburization is possible in order to obtain case hardness more than Rc65 for smaller sections that reduces with an increase in section size. Core strength will remain as it has been supplied for all the sections. Alternatively, carbon nitriding can be performed, offering certain benefits over standard carburizing. AISI 1020 steel can be largely utilized in all industrial sectors in order to enhance weldability or machinability properties. It is used in a variety of applications due to its cold drawn or turned and polished finish property.
Chemical Composition The chemical composition of AISI 1020 steel is: Element
0.17 - 0.230 %
99.08 - 99.53 %
0.30 - 0.60 %
≤ 0.040 %
≤ 0.050 %
Physical Properties The physical properties of AISI 1020 steel are: Physical Properties Density
Mechanical Properties The mechanical properties of AISI 1020 steel are:
Hardness, Knoop (Converted from Brinell hardness)
Hardness, Rockwell B(Converted from Brinell hardness)
Hardness, Vickers (Converted from Brinell hardness)
Tensile Strength, Ultimate
Tensile Strength, Yield
Elongation at Break (in 50 mm)
Reduction of Area
Modulus of Elasticity (Typical for steel)
Bulk Modulus (Typical for steel)
@Temperature -30.0 °C/-22.0 °F
@Temperature -18.0 °C/-0.400 °F
@Temperature -3.00 °C/26.6 °F
@Temperature 10.0 °C/50.0 °F
@Temperature 38.0 °C/100 °F
@Temperature 65.0 °C/149 °F
@Temperature 95.0 °C/203 °F
@Temperature 150 °C/302 °F
Poissons Ratio Charpy Impact
Shear Modulus (Typical for steel)
Machining In the cold drawn or turned and polished condition, AISI 1020 steel has high machinability. As per recommendations of machine manufacturers, AISI 1020 steel can be used for drilling, turning, milling and tapping operations using suitable feeds, tool type and speeds.
Weldability AISI 1020 can be welded by performing the most common welding processes. In the cold drawn or turned and polished condition, it has better weldability. It has been suggested that the welding process should not be performed in heat treated or carburized condition.
Heat Treatment Annealing AISI 1020 steel is heated at 870°C - 910°C followed by holding for certain time until the temperature remains constant all over the section. It is then cooled in a furnace.
Carburizing AISI 1020 is heated to between 880°C - 920°C in a suitable carburizing atmosphere followed by holding for sufficient amount of time to produce the needed carbon content and case depth. After this, refining/hardening and tempering processes are carried out to optimize the core and case properties.
Core Refining AISI 1020 steel is slowly cooled and re-heated at 870°C - 900°C followed by holding until the temperature remains constant all over the section and quenching in water, oil or brine.
Case Hardening After performing the core refining process, it is re-heated to 760°C - 780°C followed by holding until the temperature is consistent all over the section. It is then quenched in water.
Tempering AISI 1020 steel is re-heated at 150°C - 200°C followed by holding for certain time until the temperature remains constant throughout the section. It is soaked for 1 hour per 25 mm of section and then cooled under normal atmosphere. By performing the tempering process, the toughness of the case will be improved and grinding cracks will be reduced.
Normalizing AISI 1020 steel is heated at 890°C - 940°C followed by holding until the temperature remains constant throughout the section. It is soaked for 10 - 15 minutes and then cooled in still air.
Stress Relieving AISI 1020 steel is heated to 650°C - 700°C followed by holding until the temperature remains constant all over the section and soaking for 1 hour per 25 mm of section. It is then cooled in still air.
Applications AISI 1020 steel is used in case hardened condition. The applications of AISI 1020 steel are:
It is used for simple structural application such as cold headed bolts. AISI 1020 steel also finds use in the following components: o axles o general engineering parts and components o machinery parts o shafts o camshafts o gudgon pins o ratchets o light duty gears o worm gears and o spindles